Anisotropic inplane spin splitting in an asymmetric (001) GaAs/AlGaAs quantum well
 Huiqi Ye^{1},
 Changcheng Hu^{1, 2},
 Gang Wang^{1},
 Hongming Zhao^{1},
 Haitao Tian^{1},
 Xiuwen Zhang^{3},
 Wenxin Wang^{1} and
 Baoli Liu^{1}Email author
DOI: 10.1186/1556276X6520
© Ye et al; licensee Springer. 2011
Received: 2 June 2011
Accepted: 2 September 2011
Published: 2 September 2011
Abstract
The inplane spin splitting of conductionband electron has been investigated in an asymmetric (001) GaAs/Al_{ x }Ga_{1x }As quantum well by timeresolved Kerr rotation technique under a transverse magnetic field. The distinctive anisotropy of the spin splitting was observed while the temperature is below approximately 200 K. This anisotropy emerges from the combined effect of Dresselhaus spinorbit coupling plus asymmetric potential gradients. We also exploit the temperature dependence of spinsplitting energy. Both the anisotropy of spin splitting and the inplane effective gfactor decrease with increasing temperature.
PACS: 78.47.jm, 71.70.Ej, 75.75.+a, 72.25.Fe,
Keywords
quantum beats spinorbit coupling magnetic properties of nanostructures optical creation of spin polarizedIntroduction
The properties of spins in semiconductor materials have attracted much more attentions since the invention of spintronics and spinbased quantum information [1–3]. In those fields, the spinorbit coupling (SOC) plays a key role on the properties of spin states in bulk and lowdimensional semiconductor materials. It not only results in the zeromagnetic field spin splitting, which is the main source of the spin relaxation through D'yakonovPerel (DP) mechanism and novel phenomenon such as the generation of the spin current [4], but also significantly affects the spin splitting with an external magnetic field B > 0.
In general, the spin splitting of electron or hole at B > 0 in semiconductor is described by a finite Zeeman splitting energy and characterized by the effective gfactor, which is necessary for the spin manipulation and spinbased qubit with an external electrical/magnetic field in semiconductor. So far, the effective gfactor has been intensively investigated in many literatures during past few decades [5–13]. For conductionband electron, it is found that the effective gfactor is strongly dependent on the point group symmetry in semiconductor materials [7]. It is isotropic and independent on the orientation of applied magnetic field in GaAs bulk due to T _{d} point symmetry group. On the contrast, the effective gfactor becomes anisotropic and significantly depends on the direction of magnetic field in quantum structures such as GaAs/AlGaAs heterostructures and quantum well (QW) due to the reducing symmetry [7]. For example, where the point symmetry group is reduced to D _{2d}, in a rectangular/symmetric QW grown on the (001)orientated substrate, the effective gfactor can have different values for B applied in the direction normal to the plane of QW and for B in the plane of the QW due to the additional potential confinement: g _{ xx } = g _{ yy } ≠ g _{ zz } (x//[100]) [5–7, 10]. Furthermore, where the symmetry is reduced to C _{2v} in an asymmetric QW with the inversionasymmetric confining potentials, the effective gfactor is dependent on the direction of an applied inplane magnetic field, which results in the anisotropic Zeeman splitting [14]. Up to now, the spin splitting (Zeeman splitting) at B > 0 is considered to be only characterized by the effective gfactor. In fact, two proposals [7, 14] have been predicted that the Dresselhaus SOC significantly affects the spin splitting of electron at B > 0 plus structure inversion asymmetry. A new term, defined as ${b}_{41,2}^{6c6c}$ in Ref. [14], can result in the measurable anisotropy of the inplane spin splitting, although it is not a Zeeman term. We call it as Zeemanlike term thereinafter. The anisotropic spin splitting was measured experimentally at B > 0 with an applied external electric field to reduce the symmetry of quantum film but interpreted in terms of anisotropic effective gfactor by Oestreich et al. [9] In this Letter, we use the timeresolved Kerr rotation (TRKR) [15, 16] technique to study the inplane spin splitting via the accurate measurements of the Larmor procession frequency in a specially designed (001) GaAs/AlGaAs undoped QW with asymmetric confined barriers under an inplane magnetic field. We show that the spin splitting is found to be obviously anisotropic for B parallel to [110] and [110].
Experimental procedure
The sample on investigation here is grown on (001) oriented semiinsulating GaAs substrate by molecular beam epitaxy. It contains a 50nmwide Al_{0.28}Ga_{0.72}As barrier layer, an 8nmwide GaAs quantum well, the other sloping barrier grown with content of Al changing from 4.28% to 28% on the length of approximately 9 nm, and the barrier layer of a width 50 nm. The upper part of the structure is covered with a 5nm GaAs layer to avoid the oxidation of barrier. TRKR experiment was carried out in an Oxford magnetooptical cryostat supplied with a 7T splitcoil superconducting magnet. The sample was excited near normal incidence with a degenerate pump and delayed probe pulses from a Coherent modelocked Tisapphire laser (approximately 120 fs, 76 MHz). The center of the photon energy was tuned for the maximum Kerr rotation signal for each temperature setting. The laser beams were focused to a spot size of approximately 100 μm, and the pump and probe beams have an average power of 5.0 and 0.5 mW, respectively. The helicity of linearly polarized pump beam was modulated at 50 kHz by a photoelastic modulator for lockin detection. The temporal evolution of the electron spins, which were generated by the circularly polarized pump pulse, was recorded by measuring Kerr rotation angle θ _{K}(Δt) of the linearly polarized probe pulse while sweeping Δt.
Results and discussion
where S _{0} is the initial spin density, τ_{s} is spin lifetime, and ω the Larmor frequency. By this way, we obtain the exact value of the Larmor frequency ω and then the splitting energy ΔE _{ B//[110] } = 0.0263 meV and ΔE _{ B//[110] } = 0.0326 meV through the equation ΔE = ћω with inplane magnetic field parallel to [110] and [110], respectively. Here, we use $\left\Delta {E}_{\left[1\stackrel{\u0304}{1}0\right]}\Delta {E}_{\left[110\right]}\right\u2215\left\Delta {E}_{\left[1\stackrel{\u0304}{1}0\right]}\right$ to denote the anisotropy of the inplane spin splitting. We found that this anisotropy is more than 19% in this single asymmetric (001) GaAs/AlGaAs QW. We also checked the photogenerated spin concentration dependence of the spin splitting, which can be reached by changing the pump power. Figure 1b shows the pump power dependence of spin splitting with the magnetic fields along [110] and [110] at 1.5 K. The splitting energy slowly decreases with increasing pump power up to approximately 20 mW. The change of spitting energy is less than 7% for both curves and can be ignored. Therefore, the observed anisotropy is not relevant to the carrier concentration.
where g ^{*} is the effective gfactor, B _{//} is the inplane external magnetic field, ζ = +1 for B// [110] and ζ = 1 for B//[110], and γ is the cubic Dresselhaus constant. The Zeemanlike term ${b}_{41,2}^{6c6c}$, which is derived from firstorder perturbation theory applied to the Dresselhaus term, emerges from the combined effect of BIA and SIA [14]. It is clear that the term ${b}_{41,2}^{6c6c}$ results in the anisotropic spin splitting at B > 0. As expected in Equation 2, the measured spin splitting is linearly dependent on the magnetic field with a prefactor $G={g}^{*}{\mu}_{B}2\zeta {b}_{41,2}^{6c6c}$ for both directions of applied magnetic fields as shown in Figure 1c. The slope of the B linear dependence will allow us to obtain the value of G accurately, which are G _{[110]} = 0.0130 meV/T and ${G}_{\left[1\stackrel{\u0304}{1}0\right]}$ = 0.0162 meV/T for B along [110] and [110]. The difference of two values results from the opposite sign of prefactor ζ. According to Equation 3, ${b}_{41,2}^{6c6c}$ is found to be equal to approximately 0.8 μeV/T. As discussed above, a proper anisotropic Zeeman term, described in Equation (7.4) in Ref. [14], also produces the anisotropic spin splitting at B > 0 in an asymmetric (001) GaAs/AlGaAs QW. However, the prefactor ${z}_{41}^{6c6c}{\epsilon}_{z}$ is about 0.039 μeV/T for realistic parameters with the assumed internal electric field of approximately 50 kV/cm induced by the asymmetric potential gradients. It is about 20 times smaller comparing to the value of term ${b}_{41,2}^{6c6c}$. We conclude that the Zeemanlike term ${b}_{41,2}^{6c6c}$ is the main source of the anisotropy of spin splitting at B > 0 in an asymmetric QW. Additionally, the Rashba term also gives rise to a nontrivial splitting in the presence of a magnetic field, but the splitting is isotropic [14]. In fact, the Rashba term is considered to be very small in this work because we did not observe significantly the anisotropy of inplane spin relaxation [16] as shown in Figure 1a. It is consistent with the results of Ref. [18]. As shown in Equation 3, the Zeemanlike term ${b}_{41,2}^{6c6c}$ is proportional to the cubic Dresselhaus constant γ. Numerical calculations yields γ = 29.96 eV/Å^{3} at approximately 1.5 K. Here, we use the value of approximately 0.8 μeV/T of ${b}_{41,2}^{6c6c}$ and an electron wave function calculated by the k p method [19] in this asymmetric QW. It is in agreement with the value of 27.58 eV/Å^{3} (see Table 6.3 in Ref. [14]). The remaining deviations of γ probably result from differences between the actual and the nominal sample structures which lead to uncertainties in the calculation of the wave function asymmetry.
Conclusions
We observed the anisotropic inplane spin splitting of the conductionband electron in an asymmetric (001) GaAs/AlGaAs quantum well using TRKR technique with applied magnetic fields. It is confirmed that Dresselhaus spinorbit coupling can significantly affect the inplane spin splitting at B > 0 combining the asymmetric confinement potential via the numerical comparison with the proper anisotropic Zeeman splitting.
Abbreviations
 BIA:

bulk inversion asymmetry
 DP:

D'yakonovPerel
 QW:

quantum well
 SIA:

structure inversion asymmetry
 SOC:

spinorbit coupling
 TRKR:

timeresolved Kerr rotation.
Declarations
Acknowledgements
We acknowledge the financial support of this work from the ChineseFrench NSFCANR project (grant number 10911130356), National Science Foundation of China (grant number 10774183, 10874212), and National Basic Research Program of China (2009CB930500). One of the authors (HQ) would like to thank Prof. R. Winkler, Prof. V. K. Kalevich, and Prof. V. L. Korenev for many fruitful discussions.
Authors’ Affiliations
References
 Fabian J, MatosAbiague A, Ertler C, Stano P, Žutić I: Semiconductor spintronics. Acta Physica Slovaca 2007, 57: 565. 10.2478/v1015501000868
 Awschalom DD, Loss D, Samarth N: Semiconductor Spintronics and Quantum Computation. Heidelberg: SpringerVerlag; 2002.View Article
 Žutić I, Fabian J, Das Sarma S: Spintronics: fundamentals and applications. Rev Mod Phys 2004, 76: 323. 10.1103/RevModPhys.76.323View Article
 Sinova J, Culcer D, Niu Q, Sinitsyn NA, Jungwirth T, MacDonald AH: Universal intrinsic spin Hall effect. Phys Rev Lett 2004, 92: 126603.View Article
 Ivchenko EL, Kiselev AA: Electron g factor of quantumwell and superlattices. Sov Phys Semicond 1992, 26: 827.
 Kalevich VK, Korenev VL: Anisotropy of the electron g factor in GaAs/AlGaAs quantumwells. JETP Lett 1992, 56: 253.
 Kalevich VK, Korenev VL: Electron g factor anisotropy in asymmetric GaAs/AlGaAs quantum well. JETP Lette 1993, 57: 557.
 Oestreich M, Rühle WW: Temperature dependence of the electron Landé g factor in GaAs. Phys Rev Lett 1995, 74: 2315. 10.1103/PhysRevLett.74.2315View Article
 Oestreich M, Hallstein S, Rühle WW: Quantum beats in semiconductors. IEEE J Sel Top Quantum Electron 1996, 2: 747. 10.1109/2944.571776View Article
 Le Jeune P, Robart D, Marie X, Amand T, Brousseau M, Barrau J, Kalevich V, Rodichev D: Anisotropy of the electron Landé g factor in quantum wells. Semicond Sci Technol 1997, 12: 380. 10.1088/02681242/12/4/006View Article
 Yugova IA, Greilich A, Yakovlev DR, Kiselev AA, Bayer M, Petrov VV, Dolgikh YuK, Reuter D, Wieck AD: Universal behavior of the electron g factor in GaAs/Al _{ x } Ga _{1x } As quantum wells. Phys Rev B 2007, 75: 245302.View Article
 Zawadzki W, Pfeffer P, Bratschitsch R, Chen Z, Cundiff ST, Murdin BN, Pidgeon CR: Temperature dependence of the electron spin g factor in GaAs. Phys Rev B 2008, 78: 245203.View Article
 Hübner J, Döhrmann S, Hägele D, Oestreich M: Temperaturedependent electron Landé g factor and the interband matrix element of GaAs. Phys Rev B 2009, 79: 193307.View Article
 Winkler R: SpinOrbit Coupling Effects in 2D Electron and Hole Systems. Volume Chapter 7. Berlin: Springer; 2003.View Article
 Koopmans B, Haverkort JEM, de Jonge WJM, Karczewski G: Timeresolved magnetization modulation spectroscopy: a new probe of ultrafast spin dynamics. J Appl Phys 1999, 85: 6763. 10.1063/1.370191View Article
 Liu BL, Zhao HM, Wang J, Liu LS, Wang WX, Chen DM: Electron density dependence of inplane spin relaxation anisotropy in GaAs/AlGaAs twodimensional electron gas. Applied Phys Lett 2007, 90: 112111. 10.1063/1.2713353View Article
 Amand T, Marie X, Le Jeune P, Brousseau M, Robart D, Barrau J, Planel R: Spin quantum beats of 2D excitons. Phys Rev Lett 1997, 78: 1355. 10.1103/PhysRevLett.78.1355View Article
 Eldridge PS, Leyland WJH, Lagoudakis PG, Harley RT, Phillips RT, Winkler R, Henini M, Taylor D: Rashba conduction band spinsplitting for asymmetric quantum well potentials. Phys Rev B 2010, 82: 045317.View Article
 Xia JB: Effectivemass theory for superlattices grown on (11N)oriented substrates. Phys Rev B 1991, 43: 9856. 10.1103/PhysRevB.43.9856View Article
 Hiramoto T, Hirakawa K, Iye Y, Ikoma T: Phase coherence length of electron waves in narrow AlGaAs quantum wires fabricated by focused ion beam implantation. Appl Phys Lett 1989, 54: 2103. 10.1063/1.101177View Article
 Bäuerle C, Mallet F, Schopfer F, Mailly D, Eska G, Saminadayar L: Experimental test of numerical renormalizationgroup theory for inelastic scattering from magnetic impurities. Phys Rev Lett 2005, 95: 266805.View Article
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.